#------------------------------------------------------------------------------
#$Date: 2016-03-23 22:41:30 +0200 (Wed, 23 Mar 2016) $
#$Revision: 179488 $
#$URL: svn://www.crystallography.net/cod/cif/4/33/85/4338509.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4338509
loop_
_publ_author_name
'Tran, T. Thao'
'Halasyamani, P. Shiv'
'Rondinelli, James M.'
_publ_section_title
;
 Role of Acentric Displacements on the Crystal Structure and
 Second-Harmonic Generating Properties of RbPbCO3F and CsPbCO3F.
;
_journal_issue                   12
_journal_name_full               'Inorganic chemistry'
_journal_page_first              6241
_journal_page_last               6251
_journal_paper_doi               10.1021/ic500778n
_journal_volume                  53
_journal_year                    2014
_chemical_formula_sum            'C F O3 Pb Rb'
_chemical_formula_weight         371.67
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           187
_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_Hall  'P -6 2'
_symmetry_space_group_name_H-M   'P -6 m 2'
_atom_sites_solution_hydrogens   none
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            1
_cell_length_a                   5.3488(12)
_cell_length_b                   5.3488(12)
_cell_length_c                   4.8269(12)
_cell_measurement_reflns_used    821
_cell_measurement_temperature    213(2)
_cell_measurement_theta_max      27.42
_cell_measurement_theta_min      4.22
_cell_volume                     119.59(5)
_computing_cell_refinement       'SAINT v7.60A (Bruker-Nonius, 2013)'
_computing_data_collection       'APEX2 v2013.4-1 (Bruker-Nonius, 2013)'
_computing_data_reduction        'SAINT v7.60A (Bruker-Nonius, 2013)'
_computing_structure_refinement  'SHELXL v6.12 (G.M. Sheldrick, 1997)'
_computing_structure_solution    'SHELXS v6.12 (G.M. Sheldrick, 1997)'
_diffrn_ambient_temperature      213(2)
_diffrn_detector_area_resol_mean 4K
_diffrn_measured_fraction_theta_full 0.962
_diffrn_measured_fraction_theta_max 0.962
_diffrn_measurement_device_type  'Bruker DUO APEX II CCD'
_diffrn_measurement_method       CCD
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0244
_diffrn_reflns_av_sigmaI/netI    0.0201
_diffrn_reflns_limit_h_max       0
_diffrn_reflns_limit_h_min       -6
_diffrn_reflns_limit_k_max       6
_diffrn_reflns_limit_k_min       0
_diffrn_reflns_limit_l_max       5
_diffrn_reflns_limit_l_min       0
_diffrn_reflns_number            820
_diffrn_reflns_theta_full        27.42
_diffrn_reflns_theta_max         27.42
_diffrn_reflns_theta_min         4.22
_diffrn_standards_decay_%        0.0
_exptl_absorpt_coefficient_mu    45.287
_exptl_absorpt_correction_T_max  0.7455
_exptl_absorpt_correction_T_min  0.4553
_exptl_absorpt_correction_type   empirical
_exptl_absorpt_process_details   'SAINT v7.60A'
_exptl_crystal_colour            Colorless
_exptl_crystal_density_diffrn    5.161
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       Column
_exptl_crystal_F_000             158
_exptl_crystal_size_max          0.20
_exptl_crystal_size_mid          0.12
_exptl_crystal_size_min          0.12
_refine_diff_density_max         0.673
_refine_diff_density_min         -0.853
_refine_diff_density_rms         0.233
_refine_ls_abs_structure_details 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack   0.09(3)
_refine_ls_extinction_coef       0.081(6)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.267
_refine_ls_hydrogen_treatment    none
_refine_ls_matrix_type           full
_refine_ls_number_parameters     16
_refine_ls_number_reflns         132
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.267
_refine_ls_R_factor_all          0.0112
_refine_ls_R_factor_gt           0.0112
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0116P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0258
_refine_ls_wR_factor_ref         0.0258
_reflns_number_gt                132
_reflns_number_total             132
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic500778n_si_002.cif
_cod_data_source_block           RbPbCO3F
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Hexagonal' changed to 'hexagonal'
according to
/usr/data/users/saulius/crontab/automatic-downloads/rss-feeds/ACS/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from
2011-04-26.

'_exptl_absorpt_correction_type' value 'Empirical'
changed to 'empirical' according to
/usr/data/users/saulius/crontab/automatic-downloads/rss-feeds/ACS/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 2281 2013-09-26 08:29:07Z andrius 

 Adding full bibliography for 4338509--4338510.cif.
;
_cod_original_sg_symbol_H-M      P-6m2
_cod_database_code               4338509
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-y, x-y, z'
'-x+y, -x, z'
'x, y, -z'
'-y, x-y, -z'
'-x+y, -x, -z'
'-y, -x, z'
'-x+y, y, z'
'x, x-y, z'
'-y, -x, -z'
'-x+y, y, -z'
'x, x-y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Pb1 Pb 1.0000 1.0000 0.5000 0.0070(2) Uani 1 12 d S
Rb1 Rb 0.6667 0.3333 0.0000 0.0111(3) Uani 1 12 d S
F1 F 0.958(17) 0.979(9) 0.0000 0.020(14) Uani 0.33 4 d SP
O1 O 0.4726(6) 0.9451(12) 0.5000 0.0195(17) Uani 1 4 d S
C1 C 0.3333 0.6667 0.5000 0.011(3) Uani 1 12 d S
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
F F 0.0171 0.0103 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Rb Rb -0.9393 2.9676 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Pb Pb -3.3944 10.1111 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
F1 Pb1 F1 175.4(19) 3_676 .
F1 Pb1 F1 175.4(19) . 2_766
F1 Pb1 F1 175.4(19) 3_676 2_765
F1 Pb1 F1 171(4) 2_766 2_765
F1 Pb1 F1 171(4) 3_676 3_675
F1 Pb1 F1 175.4(19) 2_766 3_675
F1 Pb1 F1 171(4) . 1_556
F1 Pb1 F1 175.4(19) 2_765 1_556
F1 Pb1 F1 175.4(19) 3_675 1_556
F1 Pb1 O1 93.8(16) 3_676 3_565
F1 Pb1 O1 85.8(18) . 3_565
F1 Pb1 O1 90.44(18) 2_766 3_565
F1 Pb1 O1 90.44(18) 2_765 3_565
F1 Pb1 O1 93.8(16) 3_675 3_565
F1 Pb1 O1 85.8(18) 1_556 3_565
F1 Pb1 O1 85.8(17) 3_676 2_775
F1 Pb1 O1 90.44(18) . 2_775
F1 Pb1 O1 93.8(16) 2_766 2_775
F1 Pb1 O1 93.8(16) 2_765 2_775
F1 Pb1 O1 85.8(17) 3_675 2_775
F1 Pb1 O1 90.44(18) 1_556 2_775
O1 Pb1 O1 120.0 3_565 2_775
F1 Pb1 O1 90.44(18) 3_676 1_655
F1 Pb1 O1 93.8(16) . 1_655
F1 Pb1 O1 85.8(17) 2_766 1_655
F1 Pb1 O1 85.8(17) 2_765 1_655
F1 Pb1 O1 90.44(18) 3_675 1_655
F1 Pb1 O1 93.8(16) 1_556 1_655
O1 Pb1 O1 120.000(1) 3_565 1_655
O1 Pb1 O1 120.000(2) 2_775 1_655
F1 Pb1 O1 85.8(18) 3_676 3_675
F1 Pb1 O1 93.8(16) . 3_675
F1 Pb1 O1 90.44(18) 2_766 3_675
F1 Pb1 O1 90.44(18) 2_765 3_675
F1 Pb1 O1 85.8(18) 3_675 3_675
F1 Pb1 O1 93.8(16) 1_556 3_675
O1 Pb1 O1 169.1(2) 3_565 3_675
O1 Pb1 O1 49.1(2) 2_775 3_675
O1 Pb1 O1 70.9(2) 1_655 3_675
F1 Pb1 O1 90.44(17) 3_676 .
F1 Pb1 O1 85.8(17) . .
F1 Pb1 O1 93.8(16) 2_766 .
F1 Pb1 O1 93.8(16) 2_765 .
F1 Pb1 O1 90.44(17) 3_675 .
F1 Pb1 O1 85.8(17) 1_556 .
O1 Pb1 O1 49.1(2) 3_565 .
O1 Pb1 O1 70.9(2) 2_775 .
O1 Pb1 O1 169.1(2) 1_655 .
O1 Pb1 O1 120.0 3_675 .
F1 Pb1 O1 93.8(16) 3_676 2_765
F1 Pb1 O1 90.44(18) . 2_765
F1 Pb1 O1 85.8(17) 2_766 2_765
F1 Pb1 O1 85.8(17) 2_765 2_765
F1 Pb1 O1 93.8(16) 3_675 2_765
F1 Pb1 O1 90.44(18) 1_556 2_765
O1 Pb1 O1 70.9(2) 3_565 2_765
O1 Pb1 O1 169.1(2) 2_775 2_765
O1 Pb1 O1 49.1(2) 1_655 2_765
O1 Pb1 O1 120.000(1) 3_675 2_765
O1 Pb1 O1 120.000(2) . 2_765
F1 Rb1 F1 120.000(1) 3_665 2_655
F1 Rb1 F1 120.000(2) 3_665 .
F1 Rb1 F1 120.000(3) 2_655 .
F1 Rb1 F1 114(3) 2_655 1_545
F1 Rb1 F1 126(3) . 1_545
F1 Rb1 F1 114(3) 3_665 2_765
F1 Rb1 F1 126(3) 2_655 2_765
F1 Rb1 F1 120.000(1) 1_545 2_765
F1 Rb1 F1 126(3) 3_665 3_565
F1 Rb1 F1 114(3) . 3_565
F1 Rb1 F1 120.000(2) 1_545 3_565
F1 Rb1 F1 120.000(1) 2_765 3_565
F1 Rb1 O1 70.9(7) 3_665 2_765
F1 Rb1 O1 126.62(11) 2_655 2_765
F1 Rb1 O1 74.4(8) . 2_765
F1 Rb1 O1 74.4(8) 1_545 2_765
F1 Rb1 O1 70.9(7) 2_765 2_765
F1 Rb1 O1 126.62(11) 3_565 2_765
F1 Rb1 O1 74.4(8) 3_665 1_544
F1 Rb1 O1 70.9(7) 2_655 1_544
F1 Rb1 O1 126.62(11) . 1_544
F1 Rb1 O1 70.9(7) 1_545 1_544
F1 Rb1 O1 126.62(11) 2_765 1_544
F1 Rb1 O1 74.4(8) 3_565 1_544
O1 Rb1 O1 145.24(7) 2_765 1_544
F1 Rb1 O1 70.9(7) 3_665 2_764
F1 Rb1 O1 126.62(11) 2_655 2_764
F1 Rb1 O1 74.4(8) . 2_764
F1 Rb1 O1 74.4(8) 1_545 2_764
F1 Rb1 O1 70.9(7) 2_765 2_764
F1 Rb1 O1 126.62(11) 3_565 2_764
O1 Rb1 O1 106.62(18) 2_765 2_764
O1 Rb1 O1 62.32(14) 1_544 2_764
F1 Rb1 O1 74.4(8) 3_665 1_545
F1 Rb1 O1 70.9(7) 2_655 1_545
F1 Rb1 O1 126.62(11) . 1_545
F1 Rb1 O1 70.9(7) 1_545 1_545
F1 Rb1 O1 126.62(11) 2_765 1_545
F1 Rb1 O1 74.4(8) 3_565 1_545
O1 Rb1 O1 62.32(14) 2_765 1_545
O1 Rb1 O1 106.62(18) 1_544 1_545
O1 Rb1 O1 145.24(7) 2_764 1_545
F1 Rb1 O1 126.62(11) 3_665 3_565
F1 Rb1 O1 74.4(8) 2_655 3_565
F1 Rb1 O1 70.9(7) . 3_565
F1 Rb1 O1 126.62(11) 1_545 3_565
F1 Rb1 O1 74.4(8) 2_765 3_565
F1 Rb1 O1 70.9(7) 3_565 3_565
O1 Rb1 O1 62.32(14) 2_765 3_565
O1 Rb1 O1 145.24(7) 1_544 3_565
O1 Rb1 O1 145.24(7) 2_764 3_565
O1 Rb1 O1 62.32(14) 1_545 3_565
F1 Rb1 O1 126.62(11) 3_665 3_564
F1 Rb1 O1 74.4(8) 2_655 3_564
F1 Rb1 O1 70.9(7) . 3_564
F1 Rb1 O1 126.62(11) 1_545 3_564
F1 Rb1 O1 74.4(8) 2_765 3_564
F1 Rb1 O1 70.9(7) 3_565 3_564
O1 Rb1 O1 145.24(7) 2_765 3_564
O1 Rb1 O1 62.32(14) 1_544 3_564
O1 Rb1 O1 62.32(14) 2_764 3_564
O1 Rb1 O1 145.24(7) 1_545 3_564
O1 Rb1 O1 106.62(18) 3_565 3_564
F1 F1 F1 60.000(15) 3_675 2_765
F1 F1 Pb1 86.0(17) 3_675 .
F1 F1 Pb1 86.0(16) 2_765 .
F1 F1 Pb1 86.0(16) 3_675 1_554
F1 F1 Pb1 86.0(16) 2_765 1_554
Pb1 F1 Pb1 171(4) . 1_554
F1 F1 Rb1 146.8(13) 3_675 .
F1 F1 Rb1 86.8(14) 2_765 .
Pb1 F1 Rb1 92.1(8) . .
Pb1 F1 Rb1 92.1(8) 1_554 .
F1 F1 Rb1 86.8(14) 3_675 1_565
F1 F1 Rb1 146.8(14) 2_765 1_565
Pb1 F1 Rb1 92.1(8) . 1_565
Pb1 F1 Rb1 92.1(8) 1_554 1_565
Rb1 F1 Rb1 126(3) . 1_565
Pb1 F1 Rb1 85.4(19) . 1_665
Pb1 F1 Rb1 85.4(19) 1_554 1_665
Rb1 F1 Rb1 116.8(14) . 1_665
Rb1 F1 Rb1 116.8(14) 1_565 1_665
C1 O1 Pb1 95.43(12) . 1_455
C1 O1 Pb1 95.43(12) . .
Pb1 O1 Pb1 169.1(2) 1_455 .
C1 O1 Rb1 126.69(9) . 1_566
Pb1 O1 Rb1 86.76(8) 1_455 1_566
Pb1 O1 Rb1 86.76(8) . 1_566
C1 O1 Rb1 126.69(9) . 1_565
Pb1 O1 Rb1 86.76(8) 1_455 1_565
Pb1 O1 Rb1 86.76(8) . 1_565
Rb1 O1 Rb1 106.62(18) 1_566 1_565
O1 C1 O1 120.000(1) 2_665 .
O1 C1 O1 120.0 2_665 3_565
O1 C1 O1 120.000(1) . 3_565
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Pb1 F1 2.421(7) 3_676
Pb1 F1 2.421(7) .
Pb1 F1 2.421(7) 2_766
Pb1 F1 2.421(7) 2_765
Pb1 F1 2.421(7) 3_675
Pb1 F1 2.421(7) 1_556
Pb1 O1 2.6865(8) 3_565
Pb1 O1 2.6864(8) 2_775
Pb1 O1 2.6864(8) 1_655
Pb1 O1 2.6865(8) 3_675
Pb1 O1 2.6864(8) .
Pb1 O1 2.6864(8) 2_765
Rb1 F1 3.00(4) 3_665
Rb1 F1 3.00(4) 2_655
Rb1 F1 3.00(4) .
Rb1 F1 3.00(4) 1_545
Rb1 F1 3.00(4) 2_765
Rb1 F1 3.00(4) 3_565
Rb1 O1 3.010(3) 2_765
Rb1 O1 3.010(3) 1_544
Rb1 O1 3.010(3) 2_764
Rb1 O1 3.010(3) 1_545
Rb1 O1 3.010(3) 3_565
Rb1 O1 3.010(3) 3_564
F1 Pb1 2.421(7) 1_554
F1 Rb1 3.00(4) 1_565
F1 Rb1 3.28(8) 1_665
O1 C1 1.290(6) .
O1 Pb1 2.6864(8) 1_455
O1 Rb1 3.010(3) 1_566
O1 Rb1 3.010(3) 1_565
C1 O1 1.290(6) 2_665
C1 O1 1.290(6) 3_565
